#------------------------------------------------------------------------------
#$Date: 2015-05-28 11:23:04 +0300 (Thu, 28 May 2015) $
#$Revision: 137480 $
#$URL: svn://www.crystallography.net/cod/cif/7/11/72/7117216.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7117216
loop_
_publ_author_name
'Vadim M. Kovrugin'
'Marie Colmont'
'Oleg I. Siidra'
'Olivier Mentre'
'Alexander Al-Shuray'
'Vladislav V. Gurzhiy'
'Sergey V. Krivovichev'
_publ_section_title
;
 Oxocentered Cu(II) lead selenite honeycomb lattices hosting Cu(I)Cl2
 groups obtained by chemical vapor transport reactions
;
_journal_name_full               Chem.Commun.
_journal_page_first              9563
_journal_paper_doi               10.1039/C5cc01426C
_journal_volume                  51
_journal_year                    2015
_chemical_formula_moiety         'Cl8 Cu11 O16 Pb2 Se4, Cl2 Cu'
_chemical_formula_sum            'Cl10 Cu12 O16 Pb2 Se4'
_chemical_formula_weight         2103.20
_space_group_crystal_system      monoclinic
_space_group_IT_number           12
_space_group_name_Hall           '-C 2y'
_space_group_name_H-M_alt        'C 1 2/m 1'
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_hydrogens   .
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90
_cell_angle_beta                 119.3111(10)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   18.4956(4)
_cell_length_b                   6.14540(10)
_cell_length_c                   15.2985(4)
_cell_measurement_reflns_used    7087
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      32.02
_cell_measurement_theta_min      2.53
_cell_volume                     1516.25(6)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'ATOMS (Dowty, 2000)'
_computing_structure_refinement  'SHELXL-2013 (Sheldrick, 2013)'
_computing_structure_solution    'Superflip (Palatinus & Chapuis, 2007)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.989
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0245
_diffrn_reflns_av_unetI/netI     0.0279
_diffrn_reflns_laue_measured_fraction_full 0.995
_diffrn_reflns_laue_measured_fraction_max 0.989
_diffrn_reflns_limit_h_max       27
_diffrn_reflns_limit_h_min       -26
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            8423
_diffrn_reflns_point_group_measured_fraction_full 0.995
_diffrn_reflns_point_group_measured_fraction_max 0.989
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         32.039
_diffrn_reflns_theta_min         1.526
_exptl_absorpt_coefficient_mu    25.022
_exptl_absorpt_correction_T_max  0.7463
_exptl_absorpt_correction_T_min  0.4249
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'Bruker SADABS'
_exptl_crystal_colour            brown
_exptl_crystal_density_diffrn    4.607
_exptl_crystal_description       needle
_exptl_crystal_F_000             1892
_exptl_crystal_size_max          0.21
_exptl_crystal_size_mid          0.19
_exptl_crystal_size_min          0.12
_refine_diff_density_max         4.185
_refine_diff_density_min         -3.387
_refine_diff_density_rms         0.313
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.126
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     126
_refine_ls_number_reflns         2841
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.126
_refine_ls_R_factor_all          0.0294
_refine_ls_R_factor_gt           0.0275
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0360P)²+18.6394P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0769
_refine_ls_wR_factor_ref         0.0779
_reflns_Friedel_coverage         0.000
_reflns_friedel_fraction_full    .
_reflns_friedel_fraction_max     .
_reflns_number_gt                2665
_reflns_number_total             2841
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c5cc01426c2-4.cif
_cod_data_source_block           shelx_2
_cod_database_code               7117216
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Pb1 Pb 0.20355(2) 0.0000 0.36175(2) 0.01540(7) Uani 1 2 d S T P . .
Se1 Se 0.64331(4) 0.0000 0.20096(4) 0.00959(11) Uani 1 2 d S T P . .
Se2 Se 0.87176(4) 0.0000 0.29076(4) 0.00966(11) Uani 1 2 d S T P . .
Cu1 Cu 0.85347(5) -0.5000 0.17075(7) 0.01816(17) Uani 1 2 d S T P . .
Cu2 Cu -0.05966(5) -0.5000 0.04588(6) 0.01406(15) Uani 1 2 d S T P . .
Cu3 Cu 0.56832(5) -0.5000 0.46595(6) 0.01669(16) Uani 1 2 d S T P . .
Cu4 Cu 0.51435(3) -0.25442(8) 0.25651(4) 0.01166(11) Uani 1 1 d . . . . .
Cu5 Cu 0.0000 0.0000 0.0000 0.0475(5) Uani 1 4 d S T P . .
Cu6 Cu 0.5000 0.0000 0.5000 0.0404(4) Uani 1 4 d S T P . .
Cl1 Cl 0.74015(11) -0.5000 0.18655(15) 0.0262(4) Uani 1 2 d S T P . .
Cl2 Cl -0.19768(10) -0.5000 -0.00837(13) 0.0225(3) Uani 1 2 d S T P . .
Cl3 Cl 0.71055(10) -0.5000 0.56044(12) 0.0198(3) Uani 1 2 d S T P . .
Cl4 Cl 0.58684(13) 0.0000 0.44753(16) 0.0289(4) Uani 1 2 d S T P . .
Cl5 Cl -0.06204(15) 0.0000 0.08085(15) 0.0310(4) Uani 1 2 d S T P . .
O1 O 0.4396(3) 0.0000 -0.0824(3) 0.0163(9) Uani 1 2 d S T P . .
O2 O 0.61802(19) -0.2132(5) 0.2509(3) 0.0147(6) Uani 1 1 d . . . . .
O3 O 0.9063(2) -0.2142(6) 0.2533(3) 0.0196(7) Uani 1 1 d . . . . .
O4 O 0.9459(3) 0.0000 0.4153(4) 0.0204(10) Uani 1 2 d S T P . .
O5 O -0.0397(3) -0.5000 0.1795(3) 0.0096(7) Uani 1 2 d S T P . .
O6 O 0.5686(3) -0.5000 0.3418(3) 0.0097(7) Uani 1 2 d S T P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pb Pb -3.3944 10.1111 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O6 Pb1 O2 67.82(10) 3_455 8_445
O6 Pb1 O2 67.82(9) 3_455 3_455
O2 Pb1 O2 93.47(16) 8_445 3_455
O6 Pb1 Cl3 69.34(11) 3_455 3_455
O2 Pb1 Cl3 113.71(8) 8_445 3_455
O2 Pb1 Cl3 113.71(8) 3_455 3_455
O6 Pb1 Cl1 123.92(11) 3_455 3_455
O2 Pb1 Cl1 74.69(8) 8_445 3_455
O2 Pb1 Cl1 74.69(8) 3_455 3_455
Cl3 Pb1 Cl1 166.74(5) 3_455 3_455
O2 Se1 O2 101.3(2) 6 .
O2 Se1 O1 100.16(15) 6 5_655
O2 Se1 O1 100.15(15) . 5_655
O2 Se1 O5 62.60(11) 6 3
O2 Se1 O5 62.60(11) . 3
O1 Se1 O5 62.72(17) 5_655 3
O3 Se2 O3 103.0(2) . 6
O3 Se2 O4 98.50(16) . .
O3 Se2 O4 98.50(16) 6 .
O3 Se2 O6 61.66(12) . 3
O3 Se2 O6 61.66(12) 6 3
O4 Se2 O6 63.44(17) . 3
O5 Cu1 O3 78.31(11) 1_655 6_545
O5 Cu1 O3 78.31(11) 1_655 .
O3 Cu1 O3 113.2(2) 6_545 .
O5 Cu1 Cl1 171.06(14) 1_655 .
O3 Cu1 Cl1 96.92(9) 6_545 .
O3 Cu1 Cl1 96.92(9) . .
O5 Cu1 Cl2 84.11(13) 1_655 1_655
O3 Cu1 Cl2 119.25(11) 6_545 1_655
O3 Cu1 Cl2 119.25(11) . 1_655
Cl1 Cu1 Cl2 104.83(7) . 1_655
O5 Cu1 Cu4 37.72(7) 1_655 8_545
O3 Cu1 Cu4 95.82(10) 6_545 8_545
O3 Cu1 Cu4 40.60(9) . 8_545
Cl1 Cu1 Cu4 136.90(4) . 8_545
Cl2 Cu1 Cu4 104.27(4) 1_655 8_545
O5 Cu1 Cu4 37.72(7) 1_655 3_545
O3 Cu1 Cu4 40.60(9) 6_545 3_545
O3 Cu1 Cu4 95.82(10) . 3_545
Cl1 Cu1 Cu4 136.90(4) . 3_545
Cl2 Cu1 Cu4 104.27(4) 1_655 3_545
Cu4 Cu1 Cu4 62.07(3) 8_545 3_545
O5 Cu1 Cu2 36.74(13) 1_655 1_655
O3 Cu1 Cu2 98.28(9) 6_545 1_655
O3 Cu1 Cu2 98.28(9) . 1_655
Cl1 Cu1 Cu2 152.20(7) . 1_655
Cl2 Cu1 Cu2 47.37(4) 1_655 1_655
Cu4 Cu1 Cu2 64.10(2) 8_545 1_655
Cu4 Cu1 Cu2 64.10(2) 3_545 1_655
O5 Cu2 O1 170.52(19) . 3_445
O5 Cu2 O1 95.45(18) . 7_545
O1 Cu2 O1 75.1(2) 3_445 7_545
O5 Cu2 Cl2 89.14(13) . .
O1 Cu2 Cl2 100.34(14) 3_445 .
O1 Cu2 Cl2 175.41(14) 7_545 .
O5 Cu2 Cu1 37.27(13) . 1_455
O1 Cu2 Cu1 152.21(14) 3_445 1_455
O1 Cu2 Cu1 132.72(13) 7_545 1_455
Cl2 Cu2 Cu1 51.87(5) . 1_455
O5 Cu2 O2 55.29(12) . 8_445
O1 Cu2 O2 116.17(13) 3_445 8_445
O1 Cu2 O2 47.58(12) 7_545 8_445
Cl2 Cu2 O2 136.33(7) . 8_445
Cu1 Cu2 O2 89.43(6) 1_455 8_445
O5 Cu2 O2 55.29(12) . 3_445
O1 Cu2 O2 116.17(13) 3_445 3_445
O1 Cu2 O2 47.58(12) 7_545 3_445
Cl2 Cu2 O2 136.33(7) . 3_445
Cu1 Cu2 O2 89.43(6) 1_455 3_445
O2 Cu2 O2 43.94(11) 8_445 3_445
O6 Cu3 O4 173.4(2) . 7_646
O6 Cu3 O4 99.73(19) . 3_445
O4 Cu3 O4 73.7(2) 7_646 3_445
O6 Cu3 Cl3 93.80(14) . .
O4 Cu3 Cl3 92.77(15) 7_646 .
O4 Cu3 Cl3 166.47(14) 3_445 .
O6 Cu3 O3 58.71(13) . 3_445
O4 Cu3 O3 115.38(14) 7_646 3_445
O4 Cu3 O3 48.35(13) 3_445 3_445
Cl3 Cu3 O3 142.76(7) . 3_445
O6 Cu3 O3 58.71(13) . 8_445
O4 Cu3 O3 115.38(14) 7_646 8_445
O4 Cu3 O3 48.35(12) 3_445 8_445
Cl3 Cu3 O3 142.76(7) . 8_445
O3 Cu3 O3 45.18(12) 3_445 8_445
O5 Cu4 O6 175.95(15) 3 .
O5 Cu4 O2 95.37(15) 3 .
O6 Cu4 O2 86.28(15) . .
O5 Cu4 O3 81.29(15) 3 8_445
O6 Cu4 O3 97.18(16) . 8_445
O2 Cu4 O3 176.16(14) . 8_445
O5 Cu4 Cu4 144.62(10) 3 6_545
O6 Cu4 Cu4 38.36(10) . 6_545
O2 Cu4 Cu4 97.36(10) . 6_545
O3 Cu4 Cu4 84.43(10) 8_445 6_545
O5 Cu4 Cu1 37.65(12) 3 3_455
O6 Cu4 Cu1 140.62(12) . 3_455
O2 Cu4 Cu1 133.01(9) . 3_455
O3 Cu4 Cu1 43.65(10) 8_445 3_455
Cu4 Cu4 Cu1 121.034(13) 6_545 3_455
O5 Cu4 O3 122.38(13) 3 3_445
O6 Cu4 O3 58.20(13) . 3_445
O2 Cu4 O3 132.23(11) . 3_445
O3 Cu4 O3 49.48(14) 8_445 3_445
Cu4 Cu4 O3 34.94(5) 6_545 3_445
Cu1 Cu4 O3 88.70(6) 3_455 3_445
O5 Cu4 O2 55.88(12) 3 6
O6 Cu4 O2 123.62(13) . 6
O2 Cu4 O2 48.33(13) . 6
O3 Cu4 O2 129.81(11) 8_445 6
Cu4 Cu4 O2 145.69(5) 6_545 6
Cu1 Cu4 O2 89.97(5) 3_455 6
O3 Cu4 O2 177.95(9) 3_445 6
O5 Cu4 O1 54.66(13) 3 5_655
O6 Cu4 O1 128.31(14) . 5_655
O2 Cu4 O1 46.68(12) . 5_655
O3 Cu4 O1 129.48(13) 8_445 5_655
Cu4 Cu4 O1 116.26(3) 6_545 5_655
Cu1 Cu4 O1 89.61(7) 3_455 5_655
O3 Cu4 O1 134.74(8) 3_445 5_655
O2 Cu4 O1 43.68(7) 6 5_655
O5 Cu4 O4 120.65(13) 3 3_445
O6 Cu4 O4 56.59(14) . 3_445
O2 Cu4 O4 139.20(12) . 3_445
O3 Cu4 O4 44.65(13) 8_445 3_445
Cu4 Cu4 O4 65.05(3) 6_545 3_445
Cu1 Cu4 O4 84.99(7) 3_455 3_445
O3 Cu4 O4 42.97(8) 3_445 3_445
O2 Cu4 O4 138.41(7) 6 3_445
O1 Cu4 O4 174.11(10) 5_655 3_445
Cl5 Cu5 Cl5 180.0 5 .
Cl5 Cu5 O1 92.61(8) 5 7
Cl5 Cu5 O1 87.39(8) . 7
Cl5 Cu5 O1 87.39(8) 5 3_445
Cl5 Cu5 O1 92.61(8) . 3_445
O1 Cu5 O1 180.00(17) 7 3_445
Cl5 Cu5 O1 87.39(8) 5 3_455
Cl5 Cu5 O1 92.61(8) . 3_455
O1 Cu5 O1 42.89(15) 7 3_455
O1 Cu5 O1 137.11(15) 3_445 3_455
Cl5 Cu5 O1 92.61(8) 5 7_545
Cl5 Cu5 O1 87.39(8) . 7_545
O1 Cu5 O1 137.11(15) 7 7_545
O1 Cu5 O1 42.89(15) 3_445 7_545
O1 Cu5 O1 180.00(18) 3_455 7_545
Cl4 Cu6 Cl4 180.00(4) . 5_656
Cl4 Cu6 O4 90.47(8) . 7_656
Cl4 Cu6 O4 89.53(8) 5_656 7_656
Cl4 Cu6 O4 89.53(8) . 3_445
Cl4 Cu6 O4 90.47(8) 5_656 3_445
O4 Cu6 O4 180.0 7_656 3_445
Cl4 Cu6 O4 90.47(8) . 7_646
Cl4 Cu6 O4 89.53(8) 5_656 7_646
O4 Cu6 O4 137.72(16) 7_656 7_646
O4 Cu6 O4 42.28(16) 3_445 7_646
Cl4 Cu6 O4 89.53(8) . 3_455
Cl4 Cu6 O4 90.47(8) 5_656 3_455
O4 Cu6 O4 42.28(16) 7_656 3_455
O4 Cu6 O4 137.72(16) 3_445 3_455
O4 Cu6 O4 180.0 7_646 3_455
Cl4 Cu6 O3 108.70(7) . 4_656
Cl4 Cu6 O3 71.30(7) 5_656 4_656
O4 Cu6 O3 42.44(9) 7_656 4_656
O4 Cu6 O3 137.56(9) 3_445 4_656
O4 Cu6 O3 98.04(9) 7_646 4_656
O4 Cu6 O3 81.96(9) 3_455 4_656
Cl4 Cu6 O3 71.30(7) . 8_445
Cl4 Cu6 O3 108.70(7) 5_656 8_445
O4 Cu6 O3 137.56(9) 7_656 8_445
O4 Cu6 O3 42.44(9) 3_445 8_445
O4 Cu6 O3 81.96(9) 7_646 8_445
O4 Cu6 O3 98.04(9) 3_455 8_445
O3 Cu6 O3 180.0 4_656 8_445
Cl4 Cu6 O3 71.30(7) . 3_455
Cl4 Cu6 O3 108.70(7) 5_656 3_455
O4 Cu6 O3 81.96(9) 7_656 3_455
O4 Cu6 O3 98.04(9) 3_445 3_455
O4 Cu6 O3 137.56(9) 7_646 3_455
O4 Cu6 O3 42.44(9) 3_455 3_455
O3 Cu6 O3 123.85(10) 4_656 3_455
O3 Cu6 O3 56.15(10) 8_445 3_455
Cl4 Cu6 O3 108.70(7) . 7_646
Cl4 Cu6 O3 71.30(7) 5_656 7_646
O4 Cu6 O3 98.04(9) 7_656 7_646
O4 Cu6 O3 81.96(9) 3_445 7_646
O4 Cu6 O3 42.44(9) 7_646 7_646
O4 Cu6 O3 137.56(9) 3_455 7_646
O3 Cu6 O3 56.15(10) 4_656 7_646
O3 Cu6 O3 123.85(10) 8_445 7_646
O3 Cu6 O3 180.0 3_455 7_646
Cu1 Cl1 Pb1 135.84(9) . 3_545
Cu1 Cl1 O3 40.13(6) . .
Pb1 Cl1 O3 107.78(8) 3_545 .
Cu1 Cl1 O3 40.13(6) . 6_545
Pb1 Cl1 O3 107.78(8) 3_545 6_545
O3 Cl1 O3 65.63(13) . 6_545
Cu1 Cl1 O2 146.49(6) . 6_545
Pb1 Cl1 O2 43.85(6) 3_545 6_545
O3 Cl1 O2 149.25(11) . 6_545
O3 Cl1 O2 107.01(8) 6_545 6_545
Cu1 Cl1 O2 146.49(6) . .
Pb1 Cl1 O2 43.85(6) 3_545 .
O3 Cl1 O2 107.01(8) . .
O3 Cl1 O2 149.25(11) 6_545 .
O2 Cl1 O2 63.08(11) 6_545 .
Cu2 Cl2 Cu1 80.77(6) . 1_455
Cu2 Cl2 O5 40.21(9) . .
Cu1 Cl2 O5 40.55(8) 1_455 .
Cu2 Cl2 O1 36.32(8) . 3_445
Cu1 Cl2 O1 117.09(10) 1_455 3_445
O5 Cl2 O1 76.54(12) . 3_445
Cu3 Cl3 Pb1 83.89(5) . 3_545
Cu3 Cl3 O6 38.05(8) . .
Pb1 Cl3 O6 45.85(8) 3_545 .
Cu3 Cl3 O4 39.25(9) . 7_646
Pb1 Cl3 O4 123.15(10) 3_545 7_646
O6 Cl3 O4 77.30(12) . 7_646
Cu3 Cl3 O2 148.63(7) . 7_646
Pb1 Cl3 O2 115.52(7) 3_545 7_646
O6 Cl3 O2 152.02(8) . 7_646
O4 Cl3 O2 116.40(10) 7_646 7_646
Cu3 Cl3 O2 148.63(7) . 4_646
Pb1 Cl3 O2 115.52(7) 3_545 4_646
O6 Cl3 O2 152.02(8) . 4_646
O4 Cl3 O2 116.40(10) 7_646 4_646
O2 Cl3 O2 46.22(11) 7_646 4_646
Cu6 Cl4 O6 105.22(8) . .
Cu6 Cl4 O6 105.22(8) . 1_565
O6 Cl4 O6 128.50(14) . 1_565
Cu5 Cl5 O3 149.69(9) . 6_455
Cu5 Cl5 O3 149.69(9) . 1_455
O3 Cl5 O3 47.83(12) 6_455 1_455
Cu5 Cl5 O5 106.73(8) . 1_565
O3 Cl5 O5 45.22(9) 6_455 1_565
O3 Cl5 O5 92.14(10) 1_455 1_565
Cu5 Cl5 O5 106.73(8) . .
O3 Cl5 O5 92.14(10) 6_455 .
O3 Cl5 O5 45.22(9) 1_455 .
O5 Cl5 O5 132.38(14) 1_565 .
Se1 O1 Cu2 128.8(3) 5_655 3
Se1 O1 Cu2 126.2(2) 5_655 7_545
Cu2 O1 Cu2 104.9(2) 3 7_545
Se1 O1 O1 177.8(4) 5_655 5_655
Cu2 O1 O1 53.43(17) 3 5_655
Cu2 O1 O1 51.51(17) 7_545 5_655
Se1 O1 O2 39.71(11) 5_655 2_655
Cu2 O1 O2 142.19(15) 3 2_655
Cu2 O1 O2 97.83(17) 7_545 2_655
O1 O1 O2 138.9(2) 5_655 2_655
Se1 O1 O2 39.71(11) 5_655 5_655
Cu2 O1 O2 142.19(15) 3 5_655
Cu2 O1 O2 97.83(17) 7_545 5_655
O1 O1 O2 138.9(2) 5_655 5_655
O2 O1 O2 60.27(18) 2_655 5_655
Se1 O1 O5 85.52(18) 5_655 7_545
Cu2 O1 O5 145.7(2) 3 7_545
Cu2 O1 O5 40.73(12) 7_545 7_545
O1 O1 O5 92.2(2) 5_655 7_545
O2 O1 O5 62.99(13) 2_655 7_545
O2 O1 O5 62.99(13) 5_655 7_545
Se1 O1 Cl2 85.48(17) 5_655 3
Cu2 O1 Cl2 43.33(10) 3 3
Cu2 O1 Cl2 148.3(2) 7_545 3
O1 O1 Cl2 96.8(2) 5_655 3
O2 O1 Cl2 109.47(15) 2_655 3
O2 O1 Cl2 109.47(15) 5_655 3
O5 O1 Cl2 171.00(19) 7_545 3
Se1 O1 Cu5 111.43(7) 5_655 3
Cu2 O1 Cu5 77.42(8) 3 3
Cu2 O1 Cu5 76.85(8) 7_545 3
O1 O1 Cu5 68.55(7) 5_655 3
O2 O1 Cu5 137.96(15) 2_655 3
O2 O1 Cu5 78.94(8) 5_655 3
O5 O1 Cu5 90.82(9) 7_545 3
Cl2 O1 Cu5 92.47(8) 3 3
Se1 O1 Cu5 111.43(7) 5_655 3_545
Cu2 O1 Cu5 77.42(8) 3 3_545
Cu2 O1 Cu5 76.85(8) 7_545 3_545
O1 O1 Cu5 68.55(7) 5_655 3_545
O2 O1 Cu5 78.94(8) 2_655 3_545
O2 O1 Cu5 137.96(15) 5_655 3_545
O5 O1 Cu5 90.82(9) 7_545 3_545
Cl2 O1 Cu5 92.47(8) 3 3_545
Cu5 O1 Cu5 137.11(15) 3 3_545
Se1 O1 Cu4 67.78(13) 5_655 2_655
Cu2 O1 Cu4 150.53(10) 3 2_655
Cu2 O1 Cu4 64.39(11) 7_545 2_655
O1 O1 Cu4 110.2(2) 5_655 2_655
O2 O1 Cu4 33.45(8) 2_655 2_655
O2 O1 Cu4 67.04(12) 5_655 2_655
O5 O1 Cu4 32.83(6) 7_545 2_655
Cl2 O1 Cu4 141.34(11) 3 2_655
Cu5 O1 Cu4 122.57(11) 3 2_655
Cu5 O1 Cu4 73.42(5) 3_545 2_655
Se1 O1 Cu4 67.78(13) 5_655 5_655
Cu2 O1 Cu4 150.53(10) 3 5_655
Cu2 O1 Cu4 64.39(11) 7_545 5_655
O1 O1 Cu4 110.2(2) 5_655 5_655
O2 O1 Cu4 67.04(12) 2_655 5_655
O2 O1 Cu4 33.45(8) 5_655 5_655
O5 O1 Cu4 32.83(6) 7_545 5_655
Cl2 O1 Cu4 141.34(11) 3 5_655
Cu5 O1 Cu4 73.42(5) 3 5_655
Cu5 O1 Cu4 122.57(11) 3_545 5_655
Cu4 O1 Cu4 52.52(6) 2_655 5_655
Se1 O2 Cu4 127.34(18) . .
Se1 O2 Pb1 130.49(16) . 3_545
Cu4 O2 Pb1 101.03(13) . 3_545
Se1 O2 O1 40.14(11) . 5_655
Cu4 O2 O1 99.87(16) . 5_655
Pb1 O2 O1 150.31(16) 3_545 5_655
Se1 O2 O2 39.33(11) . 6
Cu4 O2 O2 97.36(10) . 6
Pb1 O2 O2 136.74(8) 3_545 6
O1 O2 O2 59.86(9) 5_655 6
Se1 O2 O6 170.64(19) . .
Cu4 O2 O6 46.04(10) . .
Pb1 O2 O6 55.04(11) 3_545 .
O1 O2 O6 140.17(18) 5_655 .
O2 O2 O6 131.34(9) 6 .
Se1 O2 O5 85.94(13) . 3
Cu4 O2 O5 41.52(8) . 3
Pb1 O2 O5 142.18(14) 3_545 3
O1 O2 O5 63.19(14) 5_655 3
O2 O2 O5 62.95(7) 6 3
O6 O2 O5 87.50(13) . 3
Se1 O2 Cl3 74.41(11) . 7_646
Cu4 O2 Cl3 122.93(14) . 7_646
Pb1 O2 Cl3 70.22(8) 3_545 7_646
O1 O2 Cl3 114.40(13) 5_655 7_646
O2 O2 Cl3 66.89(6) 6 7_646
O6 O2 Cl3 103.38(14) . 7_646
O5 O2 Cl3 120.41(12) 3 7_646
Se1 O2 Cl1 84.27(11) . .
Cu4 O2 Cl1 138.47(15) . .
Pb1 O2 Cl1 61.46(7) 3_545 .
O1 O2 Cl1 88.98(12) 5_655 .
O2 O2 Cl1 121.54(6) 6 .
O6 O2 Cl1 104.85(12) . .
O5 O2 Cl1 145.72(15) 3 .
Cl3 O2 Cl1 88.23(8) 7_646 .
Se1 O2 Cu4 69.48(10) . 6
Cu4 O2 Cu4 63.06(8) . 6
Pb1 O2 Cu4 139.75(13) 3_545 6
O1 O2 Cu4 69.27(10) 5_655 6
O2 O2 Cu4 34.31(5) 6 6
O6 O2 Cu4 101.49(11) . 6
O5 O2 Cu4 33.45(6) 3 6
Cl3 O2 Cu4 87.48(8) 7_646 6
Cl1 O2 Cu4 153.59(10) . 6
Se1 O2 Cu2 69.62(10) . 3
Cu4 O2 Cu2 65.29(9) . 3
Pb1 O2 Cu2 154.81(13) 3_545 3
O1 O2 Cu2 34.59(11) 5_655 3
O2 O2 Cu2 68.03(5) 6 3
O6 O2 Cu2 107.65(13) . 3
O5 O2 Cu2 32.67(9) 3 3
Cl3 O2 Cu2 134.86(10) 7_646 3
Cl1 O2 Cu2 113.79(10) . 3
Cu4 O2 Cu2 54.98(5) 6 3
Se1 O2 O2 140.67(11) . 6_545
Cu4 O2 O2 82.64(10) . 6_545
Pb1 O2 O2 43.26(8) 3_545 6_545
O1 O2 O2 120.14(9) 5_655 6_545
O2 O2 O2 180.0 6 6_545
O6 O2 O2 48.66(9) . 6_545
O5 O2 O2 117.06(7) 3 6_545
Cl3 O2 O2 113.11(6) 7_646 6_545
Cl1 O2 O2 58.46(6) . 6_545
Cu4 O2 O2 145.69(5) 6 6_545
Cu2 O2 O2 111.97(5) 3 6_545
Se2 O3 Cu4 127.87(19) . 8_545
Se2 O3 Cu1 135.67(19) . .
Cu4 O3 Cu1 95.75(13) 8_545 .
Se2 O3 O5 171.8(2) . 1_655
Cu4 O3 O5 48.23(11) 8_545 1_655
Cu1 O3 O5 47.53(11) . 1_655
Se2 O3 O4 41.28(12) . .
Cu4 O3 O4 102.59(17) 8_545 .
Cu1 O3 O4 146.49(19) . .
O5 O3 O4 142.4(2) 1_655 .
Se2 O3 O3 38.49(12) . 6
Cu4 O3 O3 95.57(10) 8_545 6
Cu1 O3 O3 146.59(11) . 6
O5 O3 O3 133.71(10) 1_655 6
O4 O3 O3 59.26(10) . 6
Se2 O3 O6 88.01(14) . 3
Cu4 O3 O6 40.64(9) 8_545 3
Cu1 O3 O6 136.21(15) . 3
O5 O3 O6 88.81(14) 1_655 3
O4 O3 O6 65.30(15) . 3
O3 O3 O6 63.32(8) 6 3
Se2 O3 Cl1 94.09(13) . .
Cu4 O3 Cl1 138.03(14) 8_545 .
Cu1 O3 Cl1 42.95(7) . .
O5 O3 Cl1 90.22(13) 1_655 .
O4 O3 Cl1 111.03(15) . .
O3 O3 Cl1 122.82(6) 6 .
O6 O3 Cl1 170.94(16) 3 .
Se2 O3 Cl5 102.07(16) . 1_655
Cu4 O3 Cl5 58.64(10) 8_545 1_655
Cu1 O3 Cl5 93.80(12) . 1_655
O5 O3 Cl5 69.70(11) 1_655 1_655
O4 O3 Cl5 119.69(14) . 1_655
O3 O3 Cl5 66.09(6) 6 1_655
O6 O3 Cl5 69.03(11) 3 1_655
Cl1 O3 Cl5 118.94(13) . 1_655
Se2 O3 Cu3 71.19(12) . 3
Cu4 O3 Cu3 67.18(10) 8_545 3
Cu1 O3 Cu3 145.47(16) . 3
O5 O3 Cu3 109.63(15) 1_655 3
O4 O3 Cu3 35.53(11) . 3
O3 O3 Cu3 67.41(6) 6 3
O6 O3 Cu3 33.68(9) 3 3
Cl1 O3 Cu3 139.53(13) . 3
Cl5 O3 Cu3 101.19(9) 1_655 3
Se2 O3 Cu4 70.61(11) . 3
Cu4 O3 Cu4 60.63(9) 8_545 3
Cu1 O3 Cu4 142.05(15) . 3
O5 O3 Cu4 102.81(12) 1_655 3
O4 O3 Cu4 71.21(11) . 3
O3 O3 Cu4 34.94(5) 6 3
O6 O3 Cu4 33.91(6) 3 3
Cl1 O3 Cu4 154.48(13) . 3
Cl5 O3 Cu4 49.13(6) 1_655 3
Cu3 O3 Cu4 55.98(5) 3 3
Se2 O3 O3 141.51(12) . 6_545
Cu4 O3 O3 84.43(10) 8_545 6_545
Cu1 O3 O3 33.41(11) . 6_545
O5 O3 O3 46.29(10) 1_655 6_545
O4 O3 O3 120.74(10) . 6_545
O3 O3 O3 180.0 6 6_545
O6 O3 O3 116.68(8) 3 6_545
Cl1 O3 O3 57.18(6) . 6_545
Cl5 O3 O3 113.91(6) 1_655 6_545
Cu3 O3 O3 112.59(6) 3 6_545
Cu4 O3 O3 145.06(5) 3 6_545
Se2 O4 Cu3 129.2(3) . 7_646
Se2 O4 Cu3 124.5(2) . 3
Cu3 O4 Cu3 106.3(2) 7_646 3
Se2 O4 O4 176.8(4) . 5_756
Cu3 O4 O4 54.01(18) 7_646 5_756
Cu3 O4 O4 52.29(18) 3 5_756
Se2 O4 O3 40.23(11) . .
Cu3 O4 O3 142.06(16) 7_646 .
Cu3 O4 O3 96.13(17) 3 .
O4 O4 O3 137.7(2) 5_756 .
Se2 O4 O3 40.23(11) . 6
Cu3 O4 O3 142.06(16) 7_646 6
Cu3 O4 O3 96.13(17) 3 6
O4 O4 O3 137.7(2) 5_756 6
O3 O4 O3 61.5(2) . 6
Se2 O4 O6 85.59(18) . 3
Cu3 O4 O6 145.2(2) 7_646 3
Cu3 O4 O6 38.89(12) 3 3
O4 O4 O6 91.2(3) 5_756 3
O3 O4 O6 63.11(14) . 3
O3 O4 O6 63.11(14) 6 3
Se2 O4 Cl3 81.25(17) . 7_646
Cu3 O4 Cl3 47.97(11) 7_646 7_646
Cu3 O4 Cl3 154.3(2) 3 7_646
O4 O4 Cl3 102.0(2) 5_756 7_646
O3 O4 Cl3 105.90(16) . 7_646
O3 O4 Cl3 105.91(16) 6 7_646
O6 O4 Cl3 166.8(2) 3 7_646
Se2 O4 Cu6 111.10(8) . 3
Cu3 O4 Cu6 77.76(9) 7_646 3
Cu3 O4 Cu6 77.26(9) 3 3
O4 O4 Cu6 68.86(8) 5_756 3
O3 O4 Cu6 138.04(15) . 3
O3 O4 Cu6 77.89(9) 6 3
O6 O4 Cu6 90.42(9) 3 3
Cl3 O4 Cu6 94.29(8) 7_646 3
Se2 O4 Cu6 111.10(8) . 3_545
Cu3 O4 Cu6 77.76(9) 7_646 3_545
Cu3 O4 Cu6 77.26(9) 3 3_545
O4 O4 Cu6 68.86(8) 5_756 3_545
O3 O4 Cu6 77.89(9) . 3_545
O3 O4 Cu6 138.04(15) 6 3_545
O6 O4 Cu6 90.42(9) 3 3_545
Cl3 O4 Cu6 94.29(8) 7_646 3_545
Cu6 O4 Cu6 137.72(16) 3 3_545
Se2 O4 Cu4 66.57(13) . 8_545
Cu3 O4 Cu4 151.96(10) 7_646 8_545
Cu3 O4 Cu4 63.47(11) 3 8_545
O4 O4 Cu4 110.6(2) 5_756 8_545
O3 O4 Cu4 32.77(9) . 8_545
O3 O4 Cu4 65.82(12) 6 8_545
O6 O4 Cu4 32.54(7) 3 8_545
Cl3 O4 Cu4 138.14(13) 7_646 8_545
Cu6 O4 Cu4 121.34(11) 3 8_545
Cu6 O4 Cu4 74.52(5) 3_545 8_545
Se2 O4 Cu4 66.57(13) . 3
Cu3 O4 Cu4 151.96(10) 7_646 3
Cu3 O4 Cu4 63.47(11) 3 3
O4 O4 Cu4 110.6(2) 5_756 3
O3 O4 Cu4 65.82(12) . 3
O3 O4 Cu4 32.77(9) 6 3
O6 O4 Cu4 32.54(7) 3 3
Cl3 O4 Cu4 138.14(13) 7_646 3
Cu6 O4 Cu4 74.52(5) 3 3
Cu6 O4 Cu4 121.34(11) 3_545 3
Cu4 O4 Cu4 49.91(6) 8_545 3
Cu2 O5 Cu1 106.0(2) . 1_455
Cu2 O5 Cu4 115.55(13) . 8_445
Cu1 O5 Cu4 104.63(14) 1_455 8_445
Cu2 O5 Cu4 115.55(13) . 3_445
Cu1 O5 Cu4 104.63(14) 1_455 3_445
Cu4 O5 Cu4 109.2(2) 8_445 3_445
Cu2 O5 O3 124.66(16) . 1_455
Cu1 O5 O3 54.16(11) 1_455 1_455
Cu4 O5 O3 50.49(10) 8_445 1_455
Cu4 O5 O3 119.4(2) 3_445 1_455
Cu2 O5 O3 124.66(16) . 6_445
Cu1 O5 O3 54.16(11) 1_455 6_445
Cu4 O5 O3 119.4(2) 8_445 6_445
Cu4 O5 O3 50.49(10) 3_445 6_445
O3 O5 O3 87.4(2) 1_455 6_445
Cu2 O5 O2 92.04(15) . 8_445
Cu1 O5 O2 147.74(13) 1_455 8_445
Cu4 O5 O2 43.11(10) 8_445 8_445
Cu4 O5 O2 90.67(17) 3_445 8_445
O3 O5 O2 93.58(12) 1_455 8_445
O3 O5 O2 133.71(19) 6_445 8_445
Cu2 O5 O2 92.04(15) . 3_445
Cu1 O5 O2 147.74(13) 1_455 3_445
Cu4 O5 O2 90.67(17) 8_445 3_445
Cu4 O5 O2 43.11(10) 3_445 3_445
O3 O5 O2 133.71(19) 1_455 3_445
O3 O5 O2 93.58(12) 6_445 3_445
O2 O5 O2 54.11(15) 8_445 3_445
Cu2 O5 O1 43.81(13) . 7_545
Cu1 O5 O1 149.8(2) 1_455 7_545
Cu4 O5 O1 92.51(14) 8_445 7_545
Cu4 O5 O1 92.51(14) 3_445 7_545
O3 O5 O1 136.00(10) 1_455 7_545
O3 O5 O1 136.00(10) 6_445 7_545
O2 O5 O1 53.82(12) 8_445 7_545
O2 O5 O1 53.82(12) 3_445 7_545
Cu2 O5 Cl2 50.65(11) . .
Cu1 O5 Cl2 55.34(11) 1_455 .
Cu4 O5 Cl2 124.91(11) 8_445 .
Cu4 O5 Cl2 124.91(11) 3_445 .
O3 O5 Cl2 90.90(14) 1_455 .
O3 O5 Cl2 90.90(14) 6_445 .
O2 O5 Cl2 135.29(14) 8_445 .
O2 O5 Cl2 135.29(14) 3_445 .
O1 O5 Cl2 94.46(15) 7_545 .
Cu2 O5 Se1 75.57(13) . 3_445
Cu1 O5 Se1 178.4(2) 1_455 3_445
Cu4 O5 Se1 74.53(12) 8_445 3_445
Cu4 O5 Se1 74.53(12) 3_445 3_445
O3 O5 Se1 125.02(13) 1_455 3_445
O3 O5 Se1 125.02(13) 6_445 3_445
O2 O5 Se1 31.47(7) 8_445 3_445
O2 O5 Se1 31.47(7) 3_445 3_445
O1 O5 Se1 31.76(10) 7_545 3_445
Cl2 O5 Se1 126.22(14) . 3_445
Cu2 O5 Cl5 66.31(7) . 1_545
Cu1 O5 Cl5 94.17(10) 1_455 1_545
Cu4 O5 Cl5 159.14(19) 8_445 1_545
Cu4 O5 Cl5 56.13(5) 3_445 1_545
O3 O5 Cl5 147.46(16) 1_455 1_545
O3 O5 Cl5 65.08(9) 6_445 1_545
O2 O5 Cl5 117.75(13) 8_445 1_545
O2 O5 Cl5 68.49(9) 3_445 1_545
O1 O5 Cl5 74.78(8) 7_545 1_545
Cl2 O5 Cl5 73.42(8) . 1_545
Se1 O5 Cl5 86.46(8) 3_445 1_545
Cu3 O6 Cu4 114.93(14) . 6_545
Cu3 O6 Cu4 114.93(14) . .
Cu4 O6 Cu4 103.3(2) 6_545 .
Cu3 O6 Pb1 113.0(2) . 3_545
Cu4 O6 Pb1 104.77(14) 6_545 3_545
Cu4 O6 Pb1 104.77(14) . 3_545
Cu3 O6 O2 133.59(13) . .
Cu4 O6 O2 111.27(19) 6_545 .
Cu4 O6 O2 47.68(9) . .
Pb1 O6 O2 57.14(10) 3_545 .
Cu3 O6 O2 133.59(13) . 6_545
Cu4 O6 O2 47.68(9) 6_545 6_545
Cu4 O6 O2 111.27(19) . 6_545
Pb1 O6 O2 57.14(10) 3_545 6_545
O2 O6 O2 82.69(18) . 6_545
Cu3 O6 O3 87.61(15) . 3_445
Cu4 O6 O3 42.17(10) 6_545 3_445
Cu4 O6 O3 87.89(17) . 3_445
Pb1 O6 O3 146.93(12) 3_545 3_445
O2 O6 O3 126.19(18) . 3_445
O2 O6 O3 89.84(12) 6_545 3_445
Cu3 O6 O3 87.61(15) . 8_445
Cu4 O6 O3 87.89(17) 6_545 8_445
Cu4 O6 O3 42.17(10) . 8_445
Pb1 O6 O3 146.93(12) 3_545 8_445
O2 O6 O3 89.84(12) . 8_445
O2 O6 O3 126.19(18) 6_545 8_445
O3 O6 O3 53.37(16) 3_445 8_445
Cu3 O6 O4 41.38(13) . 3_445
Cu4 O6 O4 90.87(15) 6_545 3_445
Cu4 O6 O4 90.86(15) . 3_445
Pb1 O6 O4 154.3(2) 3_545 3_445
O2 O6 O4 135.54(11) . 3_445
O2 O6 O4 135.54(11) 6_545 3_445
O3 O6 O4 51.59(12) 3_445 3_445
O3 O6 O4 51.59(12) 8_445 3_445
Cu3 O6 Cl3 48.16(10) . .
Cu4 O6 Cl3 128.35(10) 6_545 .
Cu4 O6 Cl3 128.35(10) . .
Pb1 O6 Cl3 64.81(11) 3_545 .
O2 O6 Cl3 103.80(14) . .
O2 O6 Cl3 103.80(14) 6_545 .
O3 O6 Cl3 129.58(14) 3_445 .
O3 O6 Cl3 129.58(14) 8_445 .
O4 O6 Cl3 89.54(15) 3_445 .
Cu3 O6 Se2 72.35(13) . 3_445
Cu4 O6 Se2 72.17(12) 6_545 3_445
Cu4 O6 Se2 72.16(12) . 3_445
Pb1 O6 Se2 174.68(17) 3_545 3_445
O2 O6 Se2 119.48(13) . 3_445
O2 O6 Se2 119.48(13) 6_545 3_445
O3 O6 Se2 30.33(8) 3_445 3_445
O3 O6 Se2 30.33(8) 8_445 3_445
O4 O6 Se2 30.97(10) 3_445 3_445
Cl3 O6 Se2 120.51(13) . 3_445
Cu3 O6 Cl4 64.81(7) . 1_545
Cu4 O6 Cl4 60.85(5) 6_545 1_545
Cu4 O6 Cl4 157.73(19) . 1_545
Pb1 O6 Cl4 94.92(9) 3_545 1_545
O2 O6 Cl4 149.60(15) . 1_545
O2 O6 Cl4 70.89(8) 6_545 1_545
O3 O6 Cl4 69.86(9) 3_445 1_545
O3 O6 Cl4 117.69(13) 8_445 1_545
O4 O6 Cl4 74.83(8) 3_445 1_545
Cl3 O6 Cl4 69.58(8) . 1_545
Se2 O6 Cl4 87.37(8) 3_445 1_545
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Pb1 O6 2.361(4) 3_455
Pb1 O2 2.420(3) 8_445
Pb1 O2 2.420(3) 3_455
Pb1 Cl3 2.9783(16) 3_455
Pb1 Cl1 3.0691(18) 3_455
Se1 O2 1.694(3) 6
Se1 O2 1.694(3) .
Se1 O1 1.709(5) 5_655
Se1 O5 3.236(4) 3
Se2 O3 1.682(3) .
Se2 O3 1.682(3) 6
Se2 O4 1.718(5) .
Se2 O6 3.329(4) 3
Cu1 O5 1.914(4) 1_655
Cu1 O3 2.104(3) 6_545
Cu1 O3 2.104(3) .
Cu1 Cl1 2.2242(18) .
Cu1 Cl2 2.4220(19) 1_655
Cu1 Cu4 3.0328(9) 8_545
Cu1 Cu4 3.0328(9) 3_545
Cu1 Cu2 3.0392(11) 1_655
Cu2 O5 1.891(4) .
Cu2 O1 1.956(4) 3_445
Cu2 O1 2.007(5) 7_545
Cu2 Cl2 2.2653(18) .
Cu2 Cu1 3.0392(11) 1_455
Cu2 O2 3.502(3) 8_445
Cu2 O2 3.502(3) 3_445
Cu3 O6 1.902(4) .
Cu3 O4 1.959(4) 7_646
Cu3 O4 2.003(5) 3_445
Cu3 Cl3 2.2993(18) .
Cu3 O3 3.428(4) 3_445
Cu3 O3 3.428(4) 8_445
Cu4 O5 1.918(2) 3
Cu4 O6 1.925(3) .
Cu4 O2 1.977(3) .
Cu4 O3 1.984(3) 8_445
Cu4 Cu4 3.0183(10) 6_545
Cu4 Cu1 3.0328(9) 3_455
Cu4 O3 3.447(3) 3_445
Cu4 O2 3.479(3) 6
Cu4 O1 3.534(4) 5_655
Cu4 O4 3.577(4) 3_445
Cu5 Cl5 2.058(2) 5
Cu5 Cl5 2.058(2) .
Cu5 O1 3.3013(17) 7
Cu5 O1 3.3013(17) 3_445
Cu5 O1 3.3013(17) 3_455
Cu5 O1 3.3013(17) 7_545
Cu6 Cl4 2.118(2) .
Cu6 Cl4 2.118(2) 5_656
Cu6 O4 3.2944(18) 7_656
Cu6 O4 3.2944(17) 3_445
Cu6 O4 3.2944(17) 7_646
Cu6 O4 3.2944(18) 3_455
Cu6 O3 3.732(4) 4_656
Cu6 O3 3.732(4) 8_445
Cu6 O3 3.732(4) 3_455
Cu6 O3 3.732(4) 7_646
Cl1 Pb1 3.0691(18) 3_545
Cl1 O3 3.241(4) .
Cl1 O3 3.241(4) 6_545
Cl1 O2 3.370(3) 6_545
Cl1 O2 3.370(3) .
Cl2 Cu1 2.4220(19) 1_455
Cl2 O5 2.929(5) .
Cl2 O1 3.248(5) 3_445
Cl3 Pb1 2.9783(16) 3_545
Cl3 O6 3.080(5) .
Cl3 O4 3.092(5) 7_646
Cl3 O2 3.338(4) 7_646
Cl3 O2 3.338(4) 4_646
Cl4 O6 3.412(2) .
Cl4 O6 3.412(2) 1_565
Cl5 O3 3.248(4) 6_455
Cl5 O3 3.248(4) 1_455
Cl5 O5 3.3586(19) 1_565
Cl5 O5 3.3586(19) .
O1 Se1 1.709(5) 5_655
O1 Cu2 1.955(4) 3
O1 Cu2 2.007(5) 7_545
O1 O1 2.414(9) 5_655
O1 O2 2.609(5) 2_655
O1 O2 2.609(5) 5_655
O1 O5 2.885(6) 7_545
O1 Cl2 3.247(5) 3
O1 Cu5 3.3013(17) 3
O1 Cu5 3.3013(17) 3_545
O1 Cu4 3.534(4) 2_655
O1 Cu4 3.534(4) 5_655
O2 Pb1 2.420(3) 3_545
O2 O1 2.609(5) 5_655
O2 O2 2.620(7) 6
O2 O6 2.668(4) .
O2 O5 2.880(5) 3
O2 Cl3 3.338(4) 7_646
O2 Cu4 3.479(3) 6
O2 Cu2 3.502(3) 3
O2 O2 3.525(7) 6_545
O3 Cu4 1.984(3) 8_545
O3 O5 2.542(4) 1_655
O3 O4 2.576(5) .
O3 O3 2.633(7) 6
O3 O6 2.932(5) 3
O3 Cl5 3.248(4) 1_655
O3 Cu3 3.428(4) 3
O3 Cu4 3.447(3) 3
O3 O3 3.512(7) 6_545
O4 Cu3 1.959(4) 7_646
O4 Cu3 2.003(5) 3
O4 O4 2.376(10) 5_756
O4 O3 2.576(5) 6
O4 O6 2.986(6) 3
O4 Cl3 3.092(5) 7_646
O4 Cu6 3.2944(17) 3
O4 Cu6 3.2944(17) 3_545
O4 Cu4 3.577(4) 8_545
O4 Cu4 3.577(4) 3
O5 Cu1 1.915(4) 1_455
O5 Cu4 1.918(2) 8_445
O5 Cu4 1.918(2) 3_445
O5 O3 2.542(4) 1_455
O5 O3 2.542(4) 6_445
O5 O2 2.880(5) 8_445
O5 O2 2.880(5) 3_445
O5 O1 2.885(6) 7_545
O5 Se1 3.236(4) 3_445
O5 Cl5 3.3586(19) 1_545
O6 Cu4 1.925(3) 6_545
O6 Pb1 2.361(4) 3_545
O6 O2 2.668(4) 6_545
O6 O3 2.932(5) 3_445
O6 O3 2.932(5) 8_445
O6 O4 2.986(6) 3_445
O6 Se2 3.329(4) 3_445
O6 Cl4 3.411(2) 1_545
